**HAL Id: hal-02467848**

**https://hal.archives-ouvertes.fr/hal-02467848**

### Submitted on 5 Feb 2020

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

**Simplified stress analysis of multilayered adhesively**

**bonded structures**

### Kübra Sekmen, Eric Paroissien, Frederic Lachaud

**To cite this version:**

### Kübra Sekmen, Eric Paroissien, Frederic Lachaud. Simplified stress analysis of multilayered

### adhe-sively bonded structures. International Journal of Adhesion and Adhesives, Elsevier, 2020, 97, pp.0.

### �10.1016/j.ijadhadh.2019.102497�. �hal-02467848�

### an author's

### https://oatao.univ-toulouse.fr/25080

### https://doi.org/10.1016/j.ijadhadh.2019.102497

### Sekmen, Kübra and Paroissien, Eric and Lachaud, Frédéric Simplified stress analysis of multilayered adhesively

### bonded structures. ( In Press: 2020) International Journal of Adhesion and Adhesives, 97. ISSN 0143-7496

### Simplified stress analysis of multilayered adhesively bonded structures

### Kubra Sekmen, Eric Paroissien

*_{, Fr�ed�eric Lachaud }

*Institut Cl�ement Ader (ICA), Universit�e de Toulouse, ISAE-SUPAERO, INSA, IMT MINES ALBI, UTIII, CNRS, 3 Rue Caroline Aigle, 31400, Toulouse, France *

*Keywords: *

Multilayered bonded joint Semi-analytical resolution Macro-element

Finite element stress analysis Stress analysis

Stress distribution Linear material adhesive

A B S T R A C T

Bolting technologies have been commonly used to assemble structural members in order to carry loads. However, the main drawback of these joints is the local reduction of the strength-to-stress ratio. Compared to the bolted joints, adhesive bonding technology allows for the increase of static and fatigue strength while reducing the weight. The Finite Element (FE) method is able to address the stress analysis of bonded joints. Nevertheless, analyses based on FE models are computationally expensive. Therefore, it is profitable to develop new simplified approaches enabling extensive parametric studies. A semi-analytical technique was developed to model the joints based on the formulation of 4-node special elements, termed macro-elements, which is able to simulate an entire bonded overlap at low computational costs. In this paper, a multilayered bonded-bars and a multilayered bonded-beams macro-elements are derived from bonded-bar and bonded-beam macro-elements. 1D-bar and 1D- beam simplified stress analyses of such multilayered joints are presented in order to predict the adhesive stress distributions along the overlap. For validation purpose, the results obtained by the simplified 1D-bar and 1D- beam model are compared with the results predicted by 1D-FE models. Good agreements are shown. Finally, the parametric studies are performed in order to understand the mechanical behavior of multilayered adhesively bonded structures. This presented simplified stress analysis can be used to deduce the sizing guidelines as a consequence of these parametric studies.

**1. Introduction **

In recent years, there has been an increasing interest in the adhe-sively bonded technology for the design of lightweight structures. Compared to the conventional methods such as riveting or bolting, bonding offers better mechanical properties in terms of stiffness, static strength and fatigue strength when joining without damaging dissimilar materials such as metals and composites [1–4]. The Finite Element (FE) method is able to address the stress analysis of bonded joints. However, since analyses based on FE models are computationally expensive, it would be profitable to develop new simplified approaches enabling extensive parametric studies. Numerous studies have attempted to perform simplified stress analysis and provided accurate predictions [5–7]. In 1938, Volkersen published the first stress analysis including the deformation of the adherends by the development of a shear lag model [8]. In 1944, Goland and Reissner developed the analysis of Volkersen by the first closed-form solution of adhesive stress distribu-tions along the overlap for simply supported balanced joint made of adherend undergoing cylindrically bending [9]. The sandwich-type analysis concept was then employed by other researchers in order to

improve this initial model considering different local equilibriums, different constitutive behaviors and various geometries [10–18]. The second and third authors of the present paper and their co-workers have been working on the development of the macro-element (ME) technique for the simplified stress analysis of bonded, bolted and hybrid (bon-ded/bolted) joints [19–29]. The ME technique is a semi-analytical res-olution method inspired by the FE method and is developed to solve the system of differential equations considering the restrictions such as dissimilar adherends, various boundary conditions, and nonlinear ad-hesive material properties. A ME is then an element which includes physical properties of both adhesive layers and adherends as illustrated in Fig. 1. A number of researchers investigated the mechanism of load transfer in multilayered structures by using shear-lag theory. Nairn and Mendels proposed an optimal shear-lag method for the stress problems of the 2D planar layered structures [30]. Jiang and Peters derived a shear-lag model for 3D multilayered structures whose properties vary along the cross-section through the extension of Nairn and Mendels’ study such as smart structures with embedded sensors and actuators [31]. Viet et al. also provided a new analytical model to predict the interlaminar shear stress in adhesively bonded multilayered metal laminates for the purpose of modeling layers of piezoelectric materials

* Corresponding author.

*E-mail address: *eric.paroissien@isae-supaero.fr (E. Paroissien).

on the future energy harvesting application [32]. Recently, Pham et al. developed a FE formulation for the analysis of multilayered beams based on the principle of stationary complementary strain energy which differs from previous studies [33].

Literature reviews have indicated that plenty of models of the adhesively bonded joints have been developed to size simple configu-rations. Although the effectiveness of the adhesively bonded joint is widely known, the stress analysis and sizing methodologies of multi-layered structures have not been extensively studied. Since studies on the stress analysis and sizing of the multilayered structures are rare to find in literature, the semi-analytical analysis in applying well-known schemes and parametric studies are performed in this work.

The objectives of the present paper are to perform the simplified stress analysis of the multilayered adhesively bonded joint under the static loading and to conduct parametric studies in order to understand their effects on the mechanical behavior of such joints. First of all, simplified stress analyses based on ME technique in 1D-bar and 1D-beam framework explained. The detailed mathematical description of semi- analytical resolution is provided. Then, 1D-FE models are presented and used to validate 1D-ME models through dedicated convergence studies. Finally, the parametric studies are performed in order to un-derstand the mechanical behavior of such joints. The computations were performed thanks to house-made computer programs developed in MATLAB. Codes are provided as supplementary materials [34].

**2. Description of simplified stress analyses of multilayered **
**bonded joints **

*2.1. Overview of the macro-element technique and application *

The simplified linear elastic method is originally developed for the hybrid (bolted/bonded) joints [21,22]. The ME technique is a mathe-matical procedure inspired by the FE method. When the ME technique

takes the shape of solutions of the governing ordinary differential equations (ODEs) systems, it differs from the common FE method because of the fact that the interpolation functions are not assumed. This method allows for the resolution of the system of ODEs, which are derived from the constitutive equations of the adhesives and adherends and local equilibrium equations, under a less restricted application field of the simplifying hypotheses in terms of the geometry, material behavior, kinematics, boundary conditions and applied loads. A direct outcome is that only one ME is sufficient to mesh a complete bonded overlap. The main work is the formulation of the elementary stiffness matrix of the multilayered bonded elements. A multilayered bonded-bars and a multilayered bonded-beams MEs are derived based on the formulation of 4-nodes bonded-bar and bonded-beam elements. In this work, the formulation is based on the exponential matrix to solve the system of first order ODEs and then to derive the elementary stiffness matrix of these ODEs. As a result, in order to assess the adherend dis-placements, internal forces and adhesive stresses, an entire bonded overlap is meshed using dedicated MEs. According to FE rules, the global stiffness matrix of the complete structure is assembled from the elementary stiffness matrices of the macro-elements. Boundary condi-tions and prescribed loadings are applied through the Augmented Lagrangian Method [34]. Based on the minimization of the total po-tential energy, the linear system is solved in order to compute the

**Nomenclature and units **

*A * matrix of the system of 1st order ODE coefficients

*Ai * *extensional stiffness (N) of adherend i *

*Bi * extensional and bending coupling stiffness (N.mm) of

*adherend i *

*Di * bending stiffness (N.mm2*) of adherend i *
*Ea,i * *adhesive Young’s modulus (MPa) of adhesive i *
*Ei * *adherend Young’s modulus (MPa) of adherend i *
*Fe * vector of nodal forces

*Gi * *adhesive shear modulus (MPa) of the adhesive i *

*K*e elementary stiffness matrix of multilayered macro-element

*L * length (mm) of bonded overlap

*Me * matrix of nodal displacements

*M*i *bending moment (N.mm) in the adherend i around the z- *

direction

*Ne * matrix of nodal forces

*N*i *normal force (N) in the adherend i in the x-direction *

*P * element nodal displacement vector

*Si * *adhesive peel stress (MPa) in the adhesive i in the y- *

direction

*S*max maximal adhesive peel stress (MPa)

*Ti * *adhesive shear stress (MPa) in the adhesive i in the x- *

direction

*T*max maximal adhesive shear stress (MPa)

*U*e vector of nodal displacements

*Vi * *shear force (N) in the adherend i in the y-direction *
*Z * vector of normal forces and displacements for semi-

analytical resolution

*b * width (mm) of the adherends

*ei * *thickness (mm) of adherend i *
*f * magnitude of applied tensile force (N)

*hi * *half thickness (mm) of adherend i *

*kI * adhesive elastic stiffness (MPa/mm) in the peel
*kII * adhesive elastic stiffness (MPa/mm) in shear
*ku * spring element stiffness (N/mm) along the x-axis
*kv * spring element stiffness (N/mm) along the y-axis
*nBE * number of bar or beam elements

*nME * number of macro-elements

*ti * *thickness (mm) of the adhesive layer i *

*tiFE * thickness (mm) of the adhesive layer used in the FE model
*ui * *displacement (mm) of adherend iin the xdirection *
*vi * *displacement (mm) of adherend iin the ydirection *

Δ*i * overlap length (mm) of a macro-element
*θi * *bending angle (rad) of the adherend iaround the *

*z-direction *

*φ _{A }* vector of normal forces and displacements at each

extremity

*φ _{F }* vector of normal forces each extremity

*φ*vector of displacements at each extremity

_{U }*νa;i * Poisson’s ratio of the adhesive layers

ð*x;y;zÞ* global reference system of axes

FE Finite Element ME macro-element

ODE ordinary differential equation

displacements and forces in the adherends as well as the adhesive shear and peel stresses. Finally, different mechanical loading could be easily taken into account.

*2.2. D-bar and 1D-beam element model *
*2.2.1. Bonded-bars element: 1D-bar kinematics *

The following hypotheses were taken (i) the adherends are linear elastic materials simulated as 1D-bars, (ii) the adhesive layer is simu-lated by an infinite number of linear elastic shear springs linking the adherends (iii) the thickness of the adhesive layer is constant along the overlap, and (iv) the adhesive stresses are constant through the thickness [8]. As a consequence of the simplified hypotheses, the following ar-guments are taken into consideration (i) only normal forces and only longitudinal displacements are considered in the adherend, (ii) the ad-hesive normal stress cannot be represented because any normal force is

not applied to the adhesive layer, and (iii) it is assumed that all the
adhesive stress components disappear except the in-plane shear. The ME
*is formed of a total of Padherends which are linked by P 1interfaces *
representing adhesive layers. The nomenclature of ME for a
multilay-ered adhesively bonded joint is described as shown in Fig. 2. The nodes
of the ME are located on the neutral axis of each layer. Each layer has 2
nodes which are located on the starting and end of the layers. Thus, a ME
*including Players has 2Pnodes in total. Within the scope of 1D-bar *
ki-nematics, there is 1�_{of freedom which is longitudinal displacement. The }

total number of degrees of freedom is computed by multiplying a total of
*nodes with a degree of freedom per nodes. As a result, 1 ME of Players *
*includes a total of 2Pdegrees of freedom. In this model, nodes at the *
interfaces are not modeled. The modeling of each layer as a bar allows
for the computation of the longitudinal displacements, normal forces,
normal stresses, and strains.

The local equilibrium of the adherends belongs to the Volkersen
type. Based on the free body diagram of infinitesimal pieces included
*between xand x þ dxof Padherends in the overlap region as presented in *

Fig. 3, one equation is obtained for each layer. As a result, a total of

*Pequations are obtained for Players. *

The local equilibrium equations are given for 1*st _{, i}th*

_{ð}

_{2 � i � P 1Þ}*and Pth*_{adherend: }
8
>
>
>
>
>
>
>
<
>
>
>
>
>
>
>
:
*dN*1
*dx* þ*T*1*b ¼ 0*
*dNi*
*dx* ð*Ti 1* *TiÞb ¼ 0*
*dNP*
*dx* *TP 1b ¼ 0*
(1)

*where Niis the normal force in the adherend i, bthe width of the *

*adherends and Ti*the adhesive shear stress.

One constitutive equation for the adhesive shear stress describes
*each interface behavior. Then, a total of P 1equations are involved. *
*For 1 � i � P* 1, the linear elastic material behavior provides the
constitutive equations of interfaces are below:

**Fig. 2. Representation of the nomenclature for the ME of multilayered joint. **

*Ti*¼

*Gi*ð*uiþ1* *ui*Þ

*ti* (2)

*where tiis the thickness of adhesive layer i, Gi*is the shear modulus of

*adhesive layer i, ui*is the normal displacement of points located at the

*abscissa xon the neutral line of adherend ibefore deformation. *
*The constitutive equations for the adherends (1 � i � P) are provided *
by:
*Ni*¼*Eibei*
*dui*
*dx* ⇒
*dui*
*dx* ¼
1
*Eibei*
*Ni* (3)

*where Eiis Young’s modulus of the adherend iand ei*the thickness of the

*adherend i. *

The ODEs are organized in order to get the expression for displace-ments and then for internal forces by the resolution. Substituting Eq. (2)

into Eq. (1), the following local equilibrium equations are obtained:
8
>
>
>
>
>
>
>
>
<
>
>
>
>
>
>
>
>
:
*dN*1
*dx* ¼*b*
*G*1
*t*1
*u*1 *b*
*G*1
*t*1
*u*2
*dNi*
*dx* ¼ *b*
*Gi 1*
*ti 1*
*ui 1*þ*b*
�
*Gi 1*
*ti 1*
þ*Gi*
*ti*
�
*ui* *b*
*Gi*
*ti*
*uiþ1*
*dNP*
*dx* ¼ *b*
*GP 1*
*tP 1*
*uP 1*þ*b*
*GP 1*
*tP 1*
*uP*
(4)

*2.2.2. Bonded-beams element: 1D-beam kinematics *

The set of simplifying hypotheses are: (i) the adherends are simulated
by linear elastic 1D Euler-Bernoulli laminated beams, (ii) the adhesive
layer is simulated by an infinite number of elastic shear and transverse
springs linking the adherends, (iii) the thickness of the adhesive layer is
constant along the overlap, and (iv) the adhesive stresses are constant
through the thickness [9]. As a consequence of the simplified hypothesis,
the following arguments are taken into consideration (i) normal forces,
shear forces and bending moments are considered in the adherends, (ii)
longitudinal displacements, deflections and bending angles are considered
in the adherends, (iii) adhesive shear and peel stresses are represented in
the adherends, and (iv) the adhesive longitudinal stresses are neglected.
*Similar to 1D-bar model, the ME is formed by Padherends and P*

1interfaces. The nomenclature of ME for a multilayered adhesively
bonded joint is presented as given in Fig. 2. Within the scope of 1D-beam
kinematics, there are 3�_{of freedom which are axial displacement, vertical }

displacement, and rotation. The total number of degrees of freedom is
computed by multiplying a total of nodes with a degree of freedom per
*nodes. As a result, one ME of Players includes a total of 6Pdegrees of *
freedom. Similar to 1D-bar model, nodes at the interfaces are not modeled
in 1D-beam model. The local equilibrium of the adherends belongs to
Goland and Reissner type. Based on the free body diagram of infinitesimal
*pieces included between xand x þ dxof Padherends in the overlap region *
as shown in Fig. 4, three equations are obtained for each layer. As a result,
*a total of 3Pequations are obtained for Players. The half thickness of the *
*adherend iare termed hi*:

*hi*¼

*ei*

2*;* *i ¼ 1; …; P* (5)

*The local equilibrium equations are given for 1st, ith*_{ð}_{2 � i � P 1Þ}*and Pth*_{adherend: }
8
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
<
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
:
*dN*1
*dx* þ*T*1*b ¼ 0*
*dV*1
*dx* *S*1*b ¼ 0*
*dM*1
*dx* þ*V*1þ*T*1*bh*1¼0
*dNi*
*dx* ð*Ti 1* *Ti*Þ*b ¼ 0*
*dVi*
*dx*þ ð*Si 1* *Si*Þ*b ¼ 0*
*dMi*
*dx* þ*Vi*þ ð*Ti 1*þ*TiÞbhi*¼0
*dNP*
*dx* *TP 1b ¼ 0*
*dVP*
*dx* þ*SP 1b ¼ 0*
*dMP*
*dx* þ*VP*þ*TP 1bhP*¼0
(6)

*where Niis the normal force in the adherend i, Vi*the shear force in the

*adherend i, Mibending moment in the adherend i, bthe width of the *

*adherend, Tithe adhesive shear stress in the adhesive iand Si*the adhesive

*peel stress in the adhesive i. *

Two constitutive equations regarding the adhesive stresses describe

*each interface behavior. Then, a total of 2ðP 1Þequations are involved. *
*For 1 � i � P* 1, the linear elastic material behavior provides the
constitutive equation of interfaces as functions of adherends
displace-ments are below:

�

*Si*¼*kI;i*ð*wi* *wiþ1*Þ

*Ti*¼*kII;iðuiþ1* *ui* *hiþ1θiþ1* *hiθiÞ* (7)
*where kI;i* ¼*E _{t}a;i*

*iis adhesive elastic stiffness in the peel, kII;i* ¼

*Gi*

*ti*adhesive

*elastic stiffness in the shear, tithe thickness of the adhesive i, Ea;i*the

*elastic modulus of the adhesive i, Githe shear modulus of the adhesive i, *
*uithe axial displacement of the adherend i, wi*the deflection of the

*adherend iand θithe bending angle of the adherend i. *

*The constitutive equations for the adherends ð1 � i � PÞare provided *
by:
8
>
>
>
>
>
>
>
<
>
>
>
>
>
>
>
:
*Ni*¼*Ai*
*dui*
*dx* *Bi*
*dθi*
*dx*⇒
*dui*
*dx*¼
*Di*
*Ωi*
*Ni*þ
*Bi*
*Ωi*
*Mi*
*Mi*¼ *Bi*
*dui*
*dx*þ*Di*
*dθi*
*dx*⇒
*dθi*
*dx* ¼
*Bi*
*Ωi*
*Ni*þ
*Ai*
*Ωi*
*Mi*
*θi*¼
*dwi*
*dx*
(8)

*where Aiis the extensional stiffness of the adherend i, Di*the bending

*stiffness of the adherend i, Bi*the extensional and bending coupling

*stiffness of the adherend iand Ωi* ¼ *AiDi*–*BiBi*is different from zero for
*i ¼ 1;…;P. *

Substituting Eq. (7) into Eq. (6), the following local equilibrium equations are obtained:

*2.3. Semi-analytical resolution *

The formulation of elementary stiffness matrices of the multilayered bonded-bars element and the multilayered bonded-beams element is derived from the linear relationship between the vector of nodal forces

*Feand the vector of the nodal displacements Ue*. The elementary stiffness

matrices for multilayered bonded-bars element and multilayered
*bonded-beams element Ke*are provided in Eqs. (10) and (11),

respectively.
0
B
B
B
B
B
@
*N*1ð0Þ
*Ni*ð0Þ
*Np*ð0Þ
*N*1ðΔÞ
*NiðΔÞ*
*NP*ðΔÞ
1
C
C
C
C
C
A
¼*Ke*
0
B
B
B
B
B
@
*u*1ð0Þ
*ui*ð0Þ
*up*ð0Þ
*u*1ðΔÞ
*uiðΔÞ*
*uP*ðΔÞ
1
C
C
C
C
C
A
*⇔ Fe*¼*KeUe* (10)

where Δis the length of the ME.

In the case of 1D-bar and 1D-beam kinematics, the semi-analytical resolution is carried out using the ME technique in order to determine the elementary stiffness matrices.

*2.4. Multilayered bonded-bars element *

The system of first order ODEs, which are derived from Eqs. (3) and (4) can be written under a matrix shape such as:

�
*dZ*
*dx*
�
¼ ½*A�fZg* (12)
*where Z ¼ ðN*1…*Ni*…*NP**u*_{1}…*ui*…*uP*Þ*T*.

The solution of the system is under the shape of the exponential of the matrix as shown in Eq. (13).

*Z ¼ expmðAxÞ:Z*0 (13)

*where fZ*0gis the vector constant.

The ME of the multilayered bonded-bars is modeled as illustrated in

Fig. 5*. From the first layer to the last layer P, all layers are assembled one *
under the other. Node numbering is provided as layer by layer in order

to obtain one multilayered ME. The numbering of degrees of freedom of
the ME is started with the first node of each layer, and it is done from the
top layer to the bottom layer. Then, after reaching the first node of the
last layer, numbering proceeds from the second nodes of the first layer to
the last layer. One multilayered bonded-bars element has a total of
*2Pnodes, 2Px1degrees of freedom, P* 1adhesive layers, and

*Padherends. *

The elementary stiffness matrix of a multilayered bonded-bars
element has to be determined. The implementation of the elementary
stiffness matrix is carried out by MATLAB software. The MATLAB
pro-vides the possibility to compute the exponential of a matrix by means of
the function “expm”. The following steps have been used to obtain the
8
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
<
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
>
:
*dN*1
*dx* ¼ *bkII;1*ð*u*2 *u*1 *h*2*θ*2 *h*1*θ*1Þ
*dV*1
*dx* ¼*bkI;1*ð*w*1 *w*2Þ
*dM*1
*dx* ¼ *V*1 *bh*1*kII;1ðu*2 *u*1 *h*2*θ*2 *h*1*θ*1Þ
*dNi*

*dx* ¼*bkII;i 1ðui* *ui 1* *hiθi* *hi 1θi 1Þ* *bkII;iðuiþ1* *ui* *hiþ1θiþ1* *hiθiÞ*
*dVi*

*dx* ¼ *bkI;i 1ðwi 1* *wiÞ þbkI;iðwi* *wiþ1Þ*
*dMi*

*dx* ¼ *Vi* *bhikII;i 1ðui* *ui 1* *hiθi* *hi 1θi 1Þ* *bhikII;iðuiþ1* *ui* *hiþ1θiþ1* *hiθ*iÞ
*dNP*
*dx* ¼*bkII;P 1ðuP* *uP 1* *hPθP* *hP 1θP 1Þ*
*dVP*
*dx* ¼ *bkI;P 1ðwP 1* *wPÞ*
*dMP*
*dx* ¼ *VP* *bhPkII;P 1ðuP* *uP 1* *hPθP* *hP 1θP 1Þ*
(9)

multilayered bonded bar element stiffness matrix. Firstly, the boundary
*conditions at both extremities of the ME in x ¼ 0and x ¼ Δlead to the *
*expressions of fundamental 6P x 6Pmatrices. *

*φA*ð*x ¼ 0Þ ¼ EXPmðAx0Þ6PX6P* (14)

*φA*ð*x ¼ ΔÞ ¼ EXPmðAxΔÞ6Px6P* (15)

Each line of these matrices indicates each line of the vector
ð*N uÞTwhich is computed at each extremity in x ¼ 0and x ¼ ΔSecondly, *
*3P x 6Pmatrices referring to displacements Uonly and forces Fonly at *
each extremity are computed.

*φU*ð0; ΔÞ ¼
�
*EXPmðAx0Þ _{i¼4P:6P;j¼1:6P}*

*EXPmðAxΔÞ*� ð

_{i¼4P:6P;j¼1:6P}*u*1ð0Þ… u

*i*ð0Þ… u

*P*ð0Þ u1ðΔÞ… u

*i*ðΔÞ… u

*P*ðΔÞÞ

*T*(16)

*φF*ð0; ΔÞ ¼ �

*EXPmðAx0Þi¼1P:3P;j¼1:6P*

*EXPmðAxΔÞ*� ð

_{i¼1P:3P;j¼1:6P}*N*1ð0Þ… N

*i*ð0Þ… N

*P*ð0Þ N1ðΔÞ… N

*i*ðΔÞ… N

*P*ðΔÞÞ

*T*(17)

*Thirdly, 6P x 6Pmatrix Me*of nodal displacements is reordered in the

base

ð*u*1ð0Þ u1ðΔÞ …uið0Þ uiðΔÞ …uPð0Þ uPðΔÞÞ*T *

*instead of ðu*1ð*0Þ… u _{i}*ð

*0Þ… u*ð

_{P}*0Þ u*

_{1}ðΔÞ…

*ui*ðΔÞ…

*uP*ðΔÞÞ

*T*.

*Me*¼ �

*EXPmðAx0Þi¼4P:6P;j¼1:6P*

*EXPmðAxΔÞ*� ð

_{i¼4P:6P;j¼1:6P}*u*1ð0Þ u1ðΔÞ …u

*i*ð0Þ u

*i*ðΔÞ …u

*P*ð0Þ u

*P*ðΔÞÞ

*T*(18)

*6P x 6Pmatrix Ne*of nodal forces is also reordered in the base

ð *N*1ð0Þ N1ðΔÞ … *Ni*ð0Þ NiðΔÞ … *NP*ð0Þ NPðΔÞÞ*T *

*instead of ðN*1ð*0Þ… N _{i}*ð

*0Þ… N*ð

_{P}*0Þ N*

_{1}ðΔÞ…

*Ni*ðΔÞ…

*NP*ðΔÞÞ

*T*.

*Ne*¼ �

*EXPmðAx0Þi¼4P:6P;j¼1:6P*

*EXPmðAxΔÞi¼4P:6P;j¼1:6P*� ð

*N*1ð0Þ N1ðΔÞ … N

*i*ð0Þ N

*i*ðΔÞ … N

*P*ð0Þ N

*P*ðΔÞÞ

*T*(19) Finally, the stiffness matrix is then computed by the following

product of matrices.

½*Ke� ¼ ½Ne�½Me�* 1 (20)

*2.4.1. Multilayered bonded-beams element *

Similar to the multilayered bonded-bars element, the system of first
order ODEs, which are derived from Eqs. (8) and (9), can be written
under a matrix shape in Eq. (12) where *Z ¼*

ð*N*_{1}…*Ni*…*NPV*1…*Vi*…*VPu*1…*ui*…*uPw*1…*wi*…*wPθ*1*…θi…θP*Þ*T*.
The solution of the system is under the shape of the exponential of
the matrix as shown in Eq. (13). The ME of the multilayered bonded-
beams is modeled as illustrated in Fig. 6. The elementary stiffness
ma-trix of a multilayered bonded-beams element has to be determined. The
following steps have been used to obtain the multilayered beam element
stiffness matrix. First of all, the boundary conditions at both extremities
*of the ME in x ¼ 0and x ¼ Δlead to the expressions of fundamental *
*6P x 6Pmatrices. *

*φA*ð*x ¼ 0Þ ¼ EXPmðAx0Þ6PX6P* (21)

*φA*ð*x ¼ ΔÞ ¼ EXPmðAxΔÞ6Px6P* (22)

Each line of these matrices indicates each line of the vector

ð*N V M u w θÞTwhich is computed at each extremity in x ¼ 0and x ¼*

Δ*Then, 3P x 6Pmatrices referring to displacements Uonly and forces *

*Fonly at each extremity are computed. *
*φU*ð0; ΔÞ ¼
�
*EXPmðAx0Þi¼4P:6P;j¼1:6P*
*EXPmðAxΔÞi¼4P:6P;j¼1:6P*
�
ð*u*0*w*0*θ*0*u*Δ*w*Δ*θ*ΔÞ*T*
(23)

**Fig. 7. Multilayered bonded joint for P ¼ 4with principle scheme of the ME. ****Table 1 **

Geometrical parameters of joint configuration.

Length of the overlap *L * 30 mm
Width of the adherends *b * 1 mm
Thickness of the adherends *ei * 2.5 mm

Thickness of the adhesives *ti * 0.11 mm

**Table 2 **

Material parameters of the adherends and adhesives.

Young’s modulus of adherends *Ei * 70 GPa

Shear modulus of the adhesives *Gi * 100 MPa

Poisson’s ratio of the adhesives *va;i * 0.3

Young’s modulus of the adhesives *Ea;i * 266 MPa

**Table 3 **

Mechanical analysis parameters.

Applied force *f * 100 N
Number of adherend layers *P * 4

*φF*ð0; ΔÞ ¼
�
*EXPmðAx0Þi¼1P:3P;j¼1:6P*
*EXPmðAxΔÞi¼1P:3P;j¼1:6P*
�
ð*N*0*V*0*M*0*N*Δ*V*Δ*M*ΔÞ*T*
(24)
*After that, 6P x 6Pmatrix Me*of nodal displacements is reordered in the

*base ðu*0*u*Δ*w*0*w*Δ*θ*0*θ*ΔÞ*Tinstead of ðu*0*w*0*θ*0*u*Δ*w*Δ*θ*ΔÞ*T*.

*Me*¼
�
*EXPmðAx0Þ _{i¼4P:6P;j¼1:6P}*

*EXPmðAxΔÞi¼4P:6P;j¼1:6P*� ð

*u*0

*u*Δ

*w*0

*w*Δ

*θ*0

*θ*ΔÞ

*T*(25)

*6P x 6Pmatrix Ne*of nodal forces is also reordered in the base

ð *N*0*N*Δ *V*0*V*Δ *M*0*M*ΔÞ*Tinstead of ðN*0*V*0*M*0*N*Δ*V*Δ*M*ΔÞ*T*.
*Ne*¼
�
*EXPmðAx0Þ _{i¼4P:6P;j¼1:6P}*

*EXPmðAxΔÞi¼4P:6P;j¼1:6P*� ð

*N*0

*N*Δ

*V*0

*V*Δ

*M*0

*M*ΔÞ

*T*(26) Finally, the stiffness matrix is then computed by the following product of matrices.

½*Ke� ¼ ½Ne*�½*Me�* 1 (27)

**3. Validation **

For validation purpose, the relevance of 1D-bar model is assessed in order to understand if the method is well-implemented. Then, the pre-dictions obtained by the simplified 1D-bar and 1D-beam ME model are compared with the results predicted by 1D-FE models.

*3.1. Nominal test case *

In this paper, a clamped-free end multilayered joint subjected to in-
*plane tensile loading with a force f. This axial force is applied to the *

*Pth _{layer at x ¼ Lwhere Lis the length of the overlap. The bonded overlap }*

*is regularly meshed with nME*of multilayered bonded-bars and

multi-layered bonded-beams elements. The number of adherends is chosen

*P ¼ 4in order to perform the stress analysis as given in *Fig. 7 with the
ME scheme. The material, geometrical and mechanical analysis
pa-rameters are provided in Tables 1–3, respectively.

*3.2. Description of the FE model *

The FE models are designed considering the same hypotheses as ME
models in order to justify the developed models [29]. This FE model is
applied to a particular case in order to study the mechanical analysis of
multilayered joints. 1D-FE models were developed by bar or beam
ele-ments for the adherends and spring element for the adhesive layers. The
nodes associated with the bar and beam elements are located at the
actual neutral line of the adherend. The nodes associated with the spring
elements are located at the actual interfaces of the adherends. Rigid
body elements are used in order to link the nodes of the neutral lines to
the nodes of the adherend interface for each adherends along the
overlaps. A scheme of the 1D-FE model is presented in Fig. 8 including
prescribed displacements and loading. It is possible to consider the
*geometrical effect of the adhesive thickness by assigning tiFE* ¼ *t _{i}*instead

*of tiFE* ¼ 0. The bar and beam elements are based on third degree
interpolating functions under the Euler-Bernoulli kinematics. The
*overlap length is regularly meshed by nBE*. The stiffnesses of springs
*ku;iand kv;i*are directly related to the mesh density along the overlap [35].

*For a spring element located at an abscissa xalong the overlap, the *
stiffnesses are computed from the actual value of adhesive peel and
*shear modulus, the adhesive thicknesses ti, the width band the mesh *

density *L*
*nBE*such as:
8
>
>
>
<
>
>
>
:
*kv;i*¼*mðxÞ*
*L*
*nBE*
*bkI;i*
*ku;i*¼*mðxÞ*
*L*
*nBE*
*bkII;i*
(28)
*where mð0 < x < LÞ ¼ 1and mðx ¼ 0Þ ¼ mðx ¼ LÞ ¼*1
2.

**Fig. 9. Maximum relative difference between FE and ME adhesive peak shear stress predictions by 1D-bar model in terms of the number of MEs used per mm. **

The FE models were developed in SAMCEF v171 FE code. All the
details and convergence studies of the FE model are available Ref. [29].
In the present paper, a number of bar or beam elements is then chosen
*equal to 600 for L ¼ 30 mmleading to a mesh density of 20 elements per *
mm providing convergent results.

*3.3. Validation of 1D-bar ME *

Before mesh influence study, the relevance of 1D-bar model is assessed in terms of the symmetry of the stiffness matrix and model restriction by a single-lap joint which has the elementary stiffness matrix determined analytically [19,22]. Firstly, the symmetry of the elemen-tary stiffness matrix is checked by computing the relative difference

between each element of the matrix and the corresponding elements of
its transpose. A maximal relative difference of 1.93 � 10 13_{% is }

computed using the geometrical and mechanical properties provided in

Tables 1–3. Secondly, the model is restricted with the single-lap joint.
The relative difference is computed 6.13 � 10 13_{% from the maximum }

difference between the elements of the stiffness matrices of the ME
model and analytical model provided in Refs. [19,22]. These small
relative differences indicate that the model is well-implemented.
Following this, the mesh influence study is studied with FE predictions
in order to justify the ME model. Mesh refinement is carried out by a
density of mesh per mm. 5 different tests are performed using 1, 2, 3, 4
*and 5 MEs per mm. The maximal adhesive shear stresses Tmax*and

*rela-tive differences between Tmax*predicted by 1D-bar ME model and those

**Fig. 11. Maximum relative difference between FE and ME adhesive peak peel stress predictions by 1D-beam model in terms of the number of MEs used per mm. **

predicted by 1D-bar FE model are provided in Table A-1 and Table A-2

(Appendix A), respectively. It can be seen in Fig. 9 that as the number of MEs per mm increases, these relative differences almost remain con-stant. A maximal relative difference of 0.02% is computed and it is observed in the 3rd adhesive layer. Figure B-1 (Appendix B) shows that the adhesive stress distributions of 1D-bar FE and 1D-bar ME models appear as superimposed along the overlap using 1 MEs per mm. Good agreement is shown because the FE model assumes the same hypotheses as the ME model. The linear elastic semi-analytical analyses are inde-pendent of the mesh refinement in the frame of 1D-bar kinematics.

*3.4. Validation of 1D-beam ME *

In the frame of 1D-beam kinematics, mesh influence study is studied
with FE predictions in order to justify the ME model. Similar to 1D-bar
ME model, mesh refinement is carried out by a density of mesh per mm.
5 different tests are performed using 1, 2, 3, 4 and 5 MEs per mm. The
*maximal adhesive shear stresses Tmaxand peel stresses Smax*and relative

*differences between Tmaxand Smax*predicted by 1D-beam ME model and

those predicted by 1D-beam FE model are provided in Tables A-3, A-4, A-5 and A-6 (Appendix A). As the number of MEs per mm increases, these relative differences firstly decrease and then almost remain

**Fig. 13. Adhesive shear stress distribution from 1D-beam ME model along the overlap. **

constant, as shown in Figs. 10 and 11. A maximal relative difference of
57.98% is computed for comparison between 1D-beam ME and FE in
*terms of Smax*and it is observed in the 1st adhesive layer with the stress

analysis of 1 ME per mm. By increasing the mesh density, this relative difference is quickly reduced to 0.09%. Figures B-2 and B-3 (Appendix B) exhibit that the adhesive stress distributions of 1D-beam FE and 1D- beam ME models appear as superimposed along the overlap using a high number of MEs per mm. The analysis results depend on the mesh refinement in the frame of 1D-beam kinematics due to the exponential matrix. Also, 1D-beam kinematics hypotheses lead to a different shape in adhesive shear stresses compared to 1D-bar kinematics.

**4. Mechanical behavior **

*4.1. Mechanical behavior (nominal test case) *

The geometrical and mechanical parameters under consideration are given in Tables 1–3. In order to understand the mechanical behavior of the adhesive layers under nominal test case conditions, the adhesive shear and peel stresses obtained with the presented 1D-bar and 1D-beam model are shown in Figs. 12–14. For the nominal test case in the frame of 1D-bar kinematics, the adhesive shear stresses along the overlap rise to a high point and peaked at the end of the overlap. The stress values of the last adhesive layer are much higher than the first and middle adhesive layers because of the chosen adherend layer for the applied force.

The presented 1D-beam model shows different adhesive shear

**Fig. 15. Adhesive peak shear stress as a function of the overlap length in the case of 1D-bar ME model. **

distribution compared to 1D-bar model due to the kinematic hypotheses taken. Fig. 13 reveals that the last adhesive layer has similar mechanical behavior whereas the adhesive shear stress distribution along the overlap of the first and the middle adhesive layer is located in the negative area. In addition, what can be clearly seen in Fig. 14 is the maximum adhesive peak peel stress in the middle adhesive layer.

*4.2. Influence of overlap length *

As an application of the simplified stress analyzed based on ME models, the influence of the overlap length on the maximal adhesive shear stress of multilayered adhesively bonded joint is studied consid-ering fixed mesh density as 10 MEs per mm. The analyses are conducted

for the overlap lengths from 10 mm to 100 mm by an increase of 10 mm.
Within 1D-bar framework, as the overlap lengths of 3 interfaces
in-crease, the maximal adhesive shear stresses inin-crease, and then tend to be
a finite value as shown in Fig. 15. Therefore, it is not useful to increase
the overlap length to decrease maximal shear stress. As Fig. 16 shows, as
the overlap length in the presented 1D-beam model increases, the
maximal adhesive shear stress of the third adhesive layer increases
*above x-axis while the maximal adhesive shear stresses of the first and *
*second adhesive layers slightly increase below x-axis. These peak shear *
stresses remain stable above a certain value of the overlap length. As for
the adhesive peak peel stresses for three adhesive layers shown in

Fig. 17*, the maximum stresses reach a peak at L ¼ 20 mm. After the *
peak, what stands out is that the maximum peel stresses decrease and

**Fig. 17. Adhesive peak peel stress as a function of the overlap length in the case of 1D-beam ME model. **

then tend to be a finite value above 30 mm. It can be concluded that it is not profitable to increase the overlap length to decrease adhesive maximal peel stress. Also, the mechanical behavior along the overlap has the same adhesive stress distributions in both 1D-bar and 1D-beam models in terms of different overlap lengths as presented in Figs. 12–14.

*4.3. Influence of adherend thickness *

The adhesive peak stresses as a function of the adherend thickness are given in Figs. 18–20. In order to understand the effect of the adherend thickness on the adhesive peak stresses, the mechanical ana-lyses are performed for different adherend thicknesses from 0.2 mm to 2 mm by an increase of 0.2 mm. For 1D-bar model shown in Fig. 18, as the thickness of the adherends increases, the peak shear stresses of all interfaces decrease and then tend to be a finite value. Therefore, it is not useful to use thicker adherends above a certain value to decrease the

maximal shear stress in the case of multilayered bonded joints. Within 1D-beam scheme, the use of thicker adherends leads to a reduction in the maximal adhesive shear stress of the three adhesive layers but then these peak stresses remain stable, as shown in Fig. 19. Fig. 20 shows that there has been a sharp increase up to 0.4 mm of adherend thickness on the maximum adhesive peel stress of second adhesive layer by increasing the adherend thickness. After reaching a peak around 0.4 mm, these maximum peel stress continuously decrease. Compared to the second adhesive layer, there has been a slight decrease in the first and third adhesive layer. After the peak value at 0.4 mm of the adherend thick-ness, maximum adhesive peel stresses fall in the three adhesive layers while the drop in the second adhesive layer is sharper than others. This non-monotonic behavior remains unexplained. It can be deduced that the maximum peel stress can be reduced by increasing the adherend thickness. In addition, for different adherend thicknesses, the stress distributions along the overlap vary as presented in Figs. 12–14.

**Fig. 19. Adhesive peak shear stress as a function of the adherend thickness in the case of 1D-beam ME model. **

**5. Conclusion **

This paper set out to perform the stress analysis of the multilayered adhesively bonded joints using a semi-analytical resolution method. The second aim of this study was to investigate the effects of the different parameters in order to understand the mechanical behavior of multi-layered adhesively bonded joints. A comparison between simplified and refined stress analyses of multilayered adhesively bonded structures subjected to pure mechanical tensile in-plane loading is presented. The simplified stress analyses are performed using 1D-bar and 1D-beam ki-nematics in order to predict the mechanical behavior of such joints. The ME technique is a semi-analytical resolution method used for the simplified stress analysis. Firstly, the simplified approach based on simplifying hypotheses is developed to model the joints. The ME tech-nique is the resolution scheme used for the simplified stress analysis. A multilayered bonded-bars and a multilayered bonded-beams MEs are derived in the frame of linear elastic adhesive behavior. The detailed mathematical derivation is presented. For the purpose of validation, the results obtained by the simplified 1D-bar and 1D-beam MEs are compared with the results predicted by 1D-FE models [29]. Mesh in-fluence studies are performed using different mesh densities in order to validate the ME mode. Relative differences between 1D-FE and 1D-ME models for different mesh densities are computed in terms of adhesive stresses. The results of this study show that the method is validated by 1D-FE model by computing small relative differences. These results, therefore, need to be interpreted with the caution that 1D-FE and 1D-ME models assume the same hypotheses and these hypotheses lead to the same results for 1D-bar model and close results for 1D-beam model. For 1D-beam model, it is found that there is a dependency on the number of MEs. Finally, parametric studies of 1D-ME models are presented con-sisting of the analysis of the influence of the overlap length and the adherend thickness. The outputs of these parametric studies are taken as adhesive peak shear and peel stresses in order to evaluate the results. The findings of this research provide insights for the computational time in the use of ME technique. This semi-analytical resolution has the advantage of the computational time for the small mesh sizes and so high number of elements through software code developed for the nu-merical analysis. Furthermore, the number of layers is not a restriction because a different number of layers are able to be simulated depending on the requirements. This presented simplified stress analysis will be of interest to deduce the sizing guidelines in order to perform the pre-liminary design. More broadly, further research in this field would be needed to determine the mechanical analysis of non-linear adhesive behavior.

**Acknowledgment **

This work has not received any specific grant.

**Appendix A. Supplementary data **

Supplementary data to this article can be found online at https://doi. org/10.1016/j.ijadhadh.2019.102497.

**References **

[1] Hart-Smith LJ. Design methodology for bonded-bolted composite joints. Volume I. Analysis derivations and illustrative solutions. California: Long Beach; 1982. [2] Higgins A. Adhesive bonding of aircraft structures. Int J Adhesion Adhes 2000;20:

367–76. https://doi.org/10.1016/S0143-7496(00)00006-3.

[3] Kelly G. Quasi-static strength and fatigue life of hybrid (bonded/bolted) composite single-lap joints. Compos Struct 2006;72:119–29. https://doi.org/10.1016/j. compstruct.2004.11.002.

[4] da Silva LFM, €Ochsner A, Adams RD. Handbook of adhesion technology. second ed., vols. 1–2. Heidelberg: Springer; 2018. https://doi.org/10.1007/978-3-319- 55411-2.

[5] van Ingen JW, Vlot A. Stress analysis of adhesively bonded single lap joints. (Report LR-740). Delft Univ Technol; 1993.

[6] Tsai MY, Morton J. An evaluation of analytical and numerical solutions to the single-lap joint. Int J Solids Struct 1994;31:2537–63. https://doi.org/10.1016/ 0020-7683(94)90036-1.

[7] da Silva LFM, das Neves PJC, Adams RD, Spelt JK. Analytical models of adhesively bonded joints - Part I: literature survey. Int J Adhesion Adhes 2009;29:319–30. https://doi.org/10.1016/j.ijadhadh.2008.06.005.

[8] Volkersen O. Die Nietkraftverteilung in zugbeanspruchten Nietverbindungen mit konstanten Laschenquerschnitten. Luftfahrtfor Schung 1938;15:41–7. [9] Goland M. The stresses in cemented joints. J Appl Mech 1944;17.

[10] Hart-Smith LJ. Adhesive-bonded scarf and stepped-lap joints. California: Long Beach; 1973.

[11] Hart-Smith LJ. Adhesive-bonded single-lap joints. California: Long Beach; 1973. [12] Hart-Smith LJ. Adhesive-bonded double-lap joints. California: Long Beach; 1973. [13] Bigwood DA, Crocombe AD. Elastic analysis and engineering design formulae for bonded joints. Int J Adhesion Adhes 1989;9:229–42. https://doi.org/10.1016/ 0143-7496(89)90066-3.

[14] Oplinger DW. A layered beam theory for single lap joints. 1991.

[15] Tsai MY, Oplinger DW, Morton J. Improved theoretical solutions for adhesive lap joints. Int J Solids Struct 1998;35:1163–85. https://doi.org/10.1016/S0020-7683 (97)00097-8.

[16] Alfredsson KS, H€ogberg JL. A closed-form solution to statically indeterminate adhesive joint problems-exemplified on ELS-specimens. Int J Adhesion Adhes 2008;28:350–61. https://doi.org/10.1016/j.ijadhadh.2007.10.002.

[17] Luo Q, Tong L. Fully-coupled nonlinear analysis of single lap adhesive joints. Int J Solids Struct 2007;44:2349–70. https://doi.org/10.1016/j.ijsolstr.2006.07.009. [18] Weißgraeber P, Stein N, Becker W. A general sandwich-type model for adhesive

joints with composite adherends. Int J Adhesion Adhes 2014;55:56–63. https:// doi.org/10.1016/j.ijadhadh.2014.06.009.

[19] Paroissien E. Contribution aux assemblages hybrides (Boulonn�es/Coll�es) – application aux jonctions a�eronautiquesvol. III. Universit�e de Toulouse; 2006. [20] Paroissien E, Sartor M, Huet J. Hybrid (bolted/bonded) joints applied to aeronautic

parts: analytical one-dimensional models of a single-lap joint. In: Tichkiewitch S, Tollenaere M, Ray P, editors. Adv. Integr. Des. Manuf. Mech. Eng. II. Dordrecht: Springer; 2007. p. 95–110.

[21] Paroissien E, Sartor M, Huet J, Lachaud F. Analytical two-dimensional model of a hybrid (Bolted/Bonded) single-lap joint. J Aircr 2007;44:573–82. https://doi.org/ 10.2514/1.24452.

[22] Paroissien E, Lachaud F, Jacobs T. A simplified stress analysis of bonded joints using macro-elements. In: Kumar S, Mittal KL, editors. Advances in modeling and design of adhesively bonded bonded systems. Adv. Model. Des. Adhes. Bond. Syst., Beverly: Wiley-Scrivener; 2013. p. 93–146. https://doi.org/10.1002/

9781118753682.

[23] Paroissien E, Gaubert F, Da Veiga A, Lachaud F. Elasto-plastic analysis of bonded joints with macro-elements. J Adhes Sci Technol 2013;27:1464–98. https://doi. org/10.1080/01694243.2012.745053.

[24] Lelias G, Paroissien E, Lachaud F, Morlier J, Schwartz S, Gavoille C. An extended semi-analytical formulation for fast and reliable mode I/II stress analysis of adhesively bonded joints. Int J Solids Struct 2015;62:18–38. https://doi.org/ 10.1016/j.ijsolstr.2014.12.027.

[25] Paroissien E, Lachaud F, Schwartz S, Da Veiga A, Barri�ere P. Simplified stress analysis of hybrid (bolted/bonded) joints. Int J Adhesion Adhes 2017;77:183–97. https://doi.org/10.1016/j.ijadhadh.2017.05.003.

[26] Paroissien E, Lachaud F, Morlier J, Schwartz S. A direct method for the assessment of cohesive zone models for thin adhesive layers loaded in mode I, mode II, and mixed-mode I/II. Rev Adhes Adhes 2018. https://doi.org/10.7569/

raa.2018.097301.

[27] Paroissien E, da Silva LFM, Lachaud F. Simplified stress analysis of functionally graded single-lap joints subjected to combined thermal and mechanical loads. Compos Struct 2018;203:85–100. https://doi.org/10.1016/j.

compstruct.2018.07.015.

[28] L�elias G, Paroissien E, Lachaud F, Morlier J. Experimental characterization of cohesive zone models for thin adhesive layers loaded in mode I, mode II, and mixed-mode I/II by the use of a direct method. Int J Solids Struct 2019;158: 90–115. https://doi.org/10.1016/j.ijsolstr.2018.09.005.

[29] Paroissien E, Lachaud F, da Silva LFM, Seddiki S. A comparison between macro- element and finite element solutions for the stress analysis of functionally graded single-lap joints. Compos Struct 2019;215:331–50. https://doi.org/10.1016/j. compstruct.2019.02.070.

[30] Nairn JA, Mendels DA. On the use of planar shear-lag methods for stress-transfer analysis of multilayered composites. Mech Mater 2001;33:335–62. https://doi. org/10.1016/S0167-6636(01)00056-4.

[31] Jiang G, Peters K. A shear-lag model for three-dimensional, unidirectional multilayered structures. Int J Solids Struct 2008;45:4049–67. https://doi.org/ 10.1016/j.ijsolstr.2008.02.018.

[32] Viet NV, Zaki W, Umer R. Interlaminar shear stress function for adhesively bonded multi-layer metal laminates. Int J Adhesion Adhes 2018;82:14–20. https://doi.org/ 10.1016/j.ijadhadh.2017.12.011.

[33] Pham P Van, Mohareb M, Fam A. Finite element formulation for the analysis of multilayered beams based on the principle of stationary complementary strain energy. Eng Struct 2018;167:287–307. https://doi.org/10.1016/j.

engstruct.2018.04.014.

[34] Simo JC, Laursen TA. An augmented Lagrangian treatment of contact problems involving friction. Comput Struct 1992;42:97–116. https://doi.org/10.1016/0045- 7949(92)90540-G.

[35] Dechwayukul C, Rubin CA, Hahn GT. Analysis of the effects of thin sealant layers in aircraft structural joints. AIAA J 2003;41:2216–28.